#------------------------------------------------------------------------------
#$Date: 2021-09-06 14:14:39 +0300 (Mon, 06 Sep 2021) $
#$Revision: 268772 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/75/7707592.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7707592
loop_
_publ_author_name
'Kuzevanova, Iryna S.'
'Kucheriv, Olesia I.'
'Hiiuk, Volodymyr M.'
'Naumova, Dina D.'
'Shova, Sergiu'
'Shylin, Sergii I.'
'Kotsyubynsky, Volodymyr O.'
'Rotaru, Aurelian'
'Fritsky, Igor O.'
'Gural'skiy, Il'ya A.'
_publ_section_title
;
 Spin crossover in iron(II) Hofmann clathrates analogues with
 1,2,3-triazole.
;
_journal_issue                   26
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              9250
_journal_page_last               9258
_journal_paper_doi               10.1039/d1dt01544c
_journal_volume                  50
_journal_year                    2021
_chemical_formula_moiety         '0.5(C16 H12 Fe2 N20 Pt2)'
_chemical_formula_sum            'C8 H6 Fe N10 Pt'
_chemical_formula_weight         493.17
_space_group_crystal_system      orthorhombic
_space_group_IT_number           74
_space_group_name_Hall           '-I 2b 2'
_space_group_name_H-M_alt        'I m m a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_audit_creation_date             2020-05-14
_audit_creation_method
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_audit_update_record
;
2021-05-12 deposited with the CCDC.	2021-06-07 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.3717(6)
_cell_length_b                   7.4268(3)
_cell_length_c                   13.1817(13)
_cell_measurement_reflns_used    902
_cell_measurement_temperature    255.00(10)
_cell_measurement_theta_max      27.8490
_cell_measurement_theta_min      2.8270
_cell_volume                     1406.96(16)
_computing_cell_refinement       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_collection       'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_data_reduction        'CrysAlisPro 1.171.39.46 (Rigaku OD, 2018)'
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      255.00(10)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 16.1593
_diffrn_detector_type            Eos
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.874
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω    -88.00 -62.00   1.00   15.00    --  -15.76-178.00 -90.00   26
  2  ω    -67.00  54.00   1.00   15.00    --  -15.76   0.00 120.00  121
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0314918000
_diffrn_orient_matrix_UB_12      -0.0019655000
_diffrn_orient_matrix_UB_13      0.0414723000
_diffrn_orient_matrix_UB_21      0.0038839000
_diffrn_orient_matrix_UB_22      0.0947187000
_diffrn_orient_matrix_UB_23      0.0050368000
_diffrn_orient_matrix_UB_31      -0.0378136000
_diffrn_orient_matrix_UB_32      0.0115376000
_diffrn_orient_matrix_UB_33      -0.0339572000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0272
_diffrn_reflns_av_unetI/netI     0.0453
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.874
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            2112
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.874
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.245
_diffrn_reflns_theta_min         2.096
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    10.969
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.66261
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.39.46 (Rigaku Oxford Diffraction, 2018)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            'clear intense colourless'
_exptl_crystal_density_diffrn    2.328
_exptl_crystal_description       plate
_exptl_crystal_F_000             912
_exptl_crystal_size_max          0.2
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.08
_refine_diff_density_max         3.618
_refine_diff_density_min         -2.035
_refine_diff_density_rms         0.246
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.062
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     57
_refine_ls_number_reflns         940
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.062
_refine_ls_R_factor_all          0.0449
_refine_ls_R_factor_gt           0.0351
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0383P)²+8.8549P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0742
_refine_ls_wR_factor_ref         0.0789
_reflns_Friedel_coverage         0.000
_reflns_number_gt                832
_reflns_number_total             940
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d1dt01544c2.cif
_cod_data_source_block           shi_4447_ilgu
_cod_depositor_comments
'Adding full bibliography for 7707591--7707592.cif.'
_cod_database_code               7707592
_shelx_shelxl_version_number     2018/1
_chemical_oxdiff_formula         Fe1Pt1C8N10H6
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.474
_shelx_estimated_absorpt_t_min   0.218
_reflns_odcompleteness_completeness 99.76
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     26.32
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All N(H) groups
2. Others
 Fixed Sof: H1A(0.25) H1B(0.25)
3.a Aromatic/amide H refined with riding coordinates:
 N3(H1A), N4(H1B), C3(H3), C2(H2)
;
_olex2_date_sample_data_collection 2019-10-10
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_oxdiff_exptl_absorpt_empirical_full_max 1.426
_oxdiff_exptl_absorpt_empirical_full_min 0.773
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y+1/2, z'
'-x, y+1/2, -z'
'x, -y, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1, z+1/2'
'-x+1/2, y+1, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'-x, -y, -z'
'x, y-1/2, -z'
'x, -y-1/2, z'
'-x, y, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y, -z+1/2'
'x+1/2, -y, z+1/2'
'-x+1/2, y+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Pt1 Pt 0.500000 0.250000 0.19521(4) 0.01685(17) Uani 1 4 d S T P . .
Fe1 Fe 0.750000 0.750000 0.250000 0.0174(4) Uani 1 4 d S T P . .
N2 N 0.6949(5) 0.750000 0.4056(6) 0.0258(17) Uani 1 2 d S T P . .
N1 N 0.6520(4) 0.5474(7) 0.2073(4) 0.0267(13) Uani 1 1 d . . . . .
N3 N 0.6073(5) 0.750000 0.4338(7) 0.033(2) Uani 1 2 d S T P . .
H1A H 0.560844 0.750000 0.392694 0.040 Uiso 0.5 2 calc RS T P A 2
C1 C 0.5972(4) 0.4396(8) 0.1991(5) 0.0187(12) Uani 1 1 d . . . . .
N4 N 0.5999(7) 0.750000 0.5324(7) 0.044(2) Uani 1 2 d S T P . .
H1B H 0.548964 0.750000 0.566585 0.052 Uiso 0.5 2 calc RS T P B 1
C3 C 0.6864(8) 0.750000 0.5706(9) 0.043(3) Uani 1 2 d S T P . .
H3 H 0.702975 0.750000 0.638834 0.051 Uiso 1 2 calc RS T P . .
C2 C 0.7439(7) 0.750000 0.4912(8) 0.040(3) Uani 1 2 d S T P . .
H2 H 0.808508 0.750000 0.495139 0.048 Uiso 1 2 calc RS T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pt Pt -1.7033 8.3905 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C1 Pt1 C1 177.0(4) . 2_655 ?
C1 Pt1 C1 89.5(3) 2_655 11_565 ?
C1 Pt1 C1 90.4(3) . 11_565 ?
C1 Pt1 C1 89.5(3) . 12_655 ?
C1 Pt1 C1 177.0(4) 12_655 11_565 ?
C1 Pt1 C1 90.4(3) 2_655 12_655 ?
N2 Fe1 N2 180.0 . 13_665 ?
N1 Fe1 N2 90.5(2) 11_575 . ?
N1 Fe1 N2 89.5(2) 11_575 13_665 ?
N1 Fe1 N2 90.5(2) 13_665 13_665 ?
N1 Fe1 N2 89.5(2) 7_645 . ?
N1 Fe1 N2 90.5(2) 7_645 13_665 ?
N1 Fe1 N2 89.5(2) . 13_665 ?
N1 Fe1 N2 89.5(2) 13_665 . ?
N1 Fe1 N2 90.5(2) . . ?
N1 Fe1 N1 90.4(3) 13_665 11_575 ?
N1 Fe1 N1 180.0 . 13_665 ?
N1 Fe1 N1 180.0(3) 11_575 7_645 ?
N1 Fe1 N1 90.4(3) . 7_645 ?
N1 Fe1 N1 89.6(3) 13_665 7_645 ?
N1 Fe1 N1 89.6(3) . 11_575 ?
N3 N2 Fe1 127.6(6) . . ?
N3 N2 C2 105.5(8) . . ?
C2 N2 Fe1 126.9(6) . . ?
C1 N1 Fe1 170.0(6) . . ?
N2 N3 H1A 124.4 . . ?
N4 N3 N2 111.1(9) . . ?
N4 N3 H1A 124.4 . . ?
N1 C1 Pt1 176.0(6) . . ?
N3 N4 H1B 126.3 . . ?
N3 N4 C3 107.4(9) . . ?
C3 N4 H1B 126.3 . . ?
N4 C3 H3 126.9 . . ?
C2 C3 N4 106.2(10) . . ?
C2 C3 H3 126.9 . . ?
N2 C2 C3 109.8(9) . . ?
N2 C2 H2 125.1 . . ?
C3 C2 H2 125.1 . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Pt1 C1 1.984(6) . ?
Pt1 C1 1.984(6) 12_655 ?
Pt1 C1 1.984(6) 2_655 ?
Pt1 C1 1.984(6) 11_565 ?
Fe1 N2 2.199(8) 13_665 ?
Fe1 N2 2.199(8) . ?
Fe1 N1 2.136(5) 7_645 ?
Fe1 N1 2.136(5) 13_665 ?
Fe1 N1 2.136(5) . ?
Fe1 N1 2.136(5) 11_575 ?
N2 N3 1.313(10) . ?
N2 C2 1.330(12) . ?
N1 C1 1.129(8) . ?
N3 H1A 0.8600 . ?
N3 N4 1.303(11) . ?
N4 H1B 0.8600 . ?
N4 C3 1.342(14) . ?
C3 H3 0.9300 . ?
C3 C2 1.333(15) . ?
C2 H2 0.9300 . ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
N3 H1A N3 0.86 2.48 3.084(15) 128.2 2_665 yes
N4 H1B N4 0.86 2.19 2.872(19) 136.5 2_665 yes
